*3.3.2 Loss of concrete's mass related to temperature*

**Figure 3** shows the evolution of mass loss during the heating cycle of the studied specimens. Before 100°C, the mass's exchange is very low. The mass loss in this temperature range corresponds mainly to the water's escape from concrete's pore, because the water chemically bound to the silicates becomes free. The chemical bonds in the C-S-H break, and the gel buildup water is released and can be evacuated.

Between 100 and 600°C, a strong mass loss for all concrete specimens was tested. Each concrete lost from 3 to 12% of its original mass. Most of the water in each concrete specimen evaporated during heating between 100 and 400°C. The increase is almost linear up to a temperature of 600°C. This is due to the evaporation of water and the progressive dehydration of C-S-H gel. Several authors, Noumowé et al., confirm that beyond 600°C, there is no more water in the concrete specimen [43, 44].

#### *3.3.3 Result of the crushing of concrete after cooling*

The compressive strength of all concrete mixtures at ambient temperature and after heating at 200, 400, 600, and 900°C is illustrated in **Figure 4**.

**115**

explained by:

*Mechanical Behavior of High-Performance Concrete under Thermal Effect*

This figure clearly shows that the compressive strength of all concrete mixtures

The concrete HPC2.5 exhibited the greatest loss in strength, about 4, 15.38, and 100% of its unheated strength when heated at 200, 600, and 900°C, respectively. We observe a stress peak at 400°C indicating a maximum value of the compressive strength of the concretes. The decomposition temperature of Ca(OH)2 varies between 400 and 600°C. If static temperature conditions are maintained, Ca(OH)2 will decompose at 400°C. This temperature seems to be the critical temperature for

Kalifa et al.'s work has shown the role of water on the performance of HPC temperature. Pressure values observed in HPC of 100–4 MPa were only 3 cm deep from the heated side to the vicinity of 250°C [46]. This further explains the prestressing

After the evaporation of physically and chemically bound water, a pressure is built up which leads to an extensive inner cracking. This inner cracking is the main reason for the reduction in strength of all concrete mixtures. Apart from it, the cement paste contracts, and aggregate expands due to loss of water at higher temperature which leads to loss of the bond between paste and aggregates.

At 900°C, we notice a low resistance for concrete with 2% adjuvant and a bursting of the concrete to those dosed of 2.5% super plasticizer (**Figure 4**). This can be

decreases at elevated temperature. According to the results obtained from the present investigation, the strength of concrete HPC2 after heated at 200, 600, and

900°C decreases by 3, 11, and 78% of its unheated strength, respectively.

force caused by the water trough described by Burlion et al. [47].

*3.3.3.1 Influence of super plasticizer on the mechanical strength*

a portland cement concrete [45].

*DOI: http://dx.doi.org/10.5772/intechopen.89916*

*Evolution of mass loss related to temperature [18].*

*Compressive strength after cooling relative the initial strength [18].*

**Figure 3.**

**Figure 4.**

**Figure 2.** *Concrete samples exposed to high temperature [18].*

*Mechanical Behavior of High-Performance Concrete under Thermal Effect DOI: http://dx.doi.org/10.5772/intechopen.89916*

**Figure 3.** *Evolution of mass loss related to temperature [18].*

*Compressive Strength of Concrete*

**3.3 Results and discussion**

*3.3.1 High-temperature effects on surface properties of concrete*

to 900°C than the ones with 400 and 600°C.

*3.3.2 Loss of concrete's mass related to temperature*

*3.3.3 Result of the crushing of concrete after cooling*

As seen in **Figure 2**, some color changes happen on the surface of concrete samples due to high temperature effects. As a result of these color changes the range of temperature values can be certainly appraised. It can be seen that cracking, rupture, and color changes happened much more in the concrete samples exposed

**Figure 3** shows the evolution of mass loss during the heating cycle of the studied specimens. Before 100°C, the mass's exchange is very low. The mass loss in this temperature range corresponds mainly to the water's escape from concrete's pore, because the water chemically bound to the silicates becomes free. The chemical bonds in the

Between 100 and 600°C, a strong mass loss for all concrete specimens was tested.

The compressive strength of all concrete mixtures at ambient temperature and

C-S-H break, and the gel buildup water is released and can be evacuated.

after heating at 200, 400, 600, and 900°C is illustrated in **Figure 4**.

Each concrete lost from 3 to 12% of its original mass. Most of the water in each concrete specimen evaporated during heating between 100 and 400°C. The increase is almost linear up to a temperature of 600°C. This is due to the evaporation of water and the progressive dehydration of C-S-H gel. Several authors, Noumowé et al., confirm that beyond 600°C, there is no more water in the concrete specimen [43, 44].

**114**

**Figure 2.**

*Concrete samples exposed to high temperature [18].*

**Figure 4.** *Compressive strength after cooling relative the initial strength [18].*

This figure clearly shows that the compressive strength of all concrete mixtures decreases at elevated temperature. According to the results obtained from the present investigation, the strength of concrete HPC2 after heated at 200, 600, and 900°C decreases by 3, 11, and 78% of its unheated strength, respectively.

The concrete HPC2.5 exhibited the greatest loss in strength, about 4, 15.38, and 100% of its unheated strength when heated at 200, 600, and 900°C, respectively. We observe a stress peak at 400°C indicating a maximum value of the compressive strength of the concretes. The decomposition temperature of Ca(OH)2 varies between 400 and 600°C. If static temperature conditions are maintained, Ca(OH)2 will decompose at 400°C. This temperature seems to be the critical temperature for a portland cement concrete [45].

Kalifa et al.'s work has shown the role of water on the performance of HPC temperature. Pressure values observed in HPC of 100–4 MPa were only 3 cm deep from the heated side to the vicinity of 250°C [46]. This further explains the prestressing force caused by the water trough described by Burlion et al. [47].

After the evaporation of physically and chemically bound water, a pressure is built up which leads to an extensive inner cracking. This inner cracking is the main reason for the reduction in strength of all concrete mixtures. Apart from it, the cement paste contracts, and aggregate expands due to loss of water at higher temperature which leads to loss of the bond between paste and aggregates.

#### *3.3.3.1 Influence of super plasticizer on the mechanical strength*

At 900°C, we notice a low resistance for concrete with 2% adjuvant and a bursting of the concrete to those dosed of 2.5% super plasticizer (**Figure 4**). This can be explained by:


## *3.3.3.2 Influence of silica fume on the mechanical strength*

In this part of the study, we want to highlight the influence of silica fume on the mechanical behavior of HPC. After the passage in the oven, the concrete specimens were cooled for 24 h in the laboratory, at a temperature of 20 ± 5°C before submitting to compressive strength test. The specimens of HPC exposed at high temperature are schematized as shown in **Figure 5**.

As expected, the replacement of cement by 5% of silica fume increased the compressive strength approximately 30% at 28 days. This is due to the reaction of the silica fume with calcium hydroxide formed during the hydration of cement that caused the formation of calcium silicate hydrate (C-S-H) as well as filler role of very fine particles of silica fume. In general, it can be concluded that concretes containing silica fume had significantly higher strength than that of CR concretes at room temperature. After exposure to 200°C, significant reductions occurred in the compressive strength of concretes without SF. Results showed the strength recovery of 18% for the concretes HPC2.5 after heating to 400°C when compared to 200°C. The compressive strength gains at 400°C are attributed to the increase in the forces between gel particles (van der Waals forces) due to the removal of water content [48].

In the range of 400–600°C, severe strength losses occurred in two concretes, HPC2.5 and CR2.5. During exposure to high temperatures, cement paste contracts, whereas aggregates expand. Thus, the transition zone and bonding between aggregates and paste are weakened. After heating to 600°C, the compressive strengths of CR were lower than those of the concretes HPC2.5. This is attributed to the presence and amount of silica fume in concretes that produced very denser transition zone between aggregates and paste due to its ultrafine particles as filler and its pozzolanic reactions.

**117**

**Figure 6.**

*Porosity as a function of temperature [18].*

weak.

*3.3.3.3 Porosity*

temperatures.

*Mechanical Behavior of High-Performance Concrete under Thermal Effect*

At 600°C, the quick losses in compressive strength for HPC2.5 concretes are attributed to the dense microstructure in this type of concretes, which caused the buildup of higher internal pressure due to the water vapor transition of the interlayer water. As a result, this process as well as chemical decomposition of hydration products causes severe deteriorations and strength loses in concrete after subjecting to high temperatures. It seems that the dosage of silica fume has no significant effect on the relative residual compressive strength at 200°C. However, between 200 and 400°C, the amount of 5% of silica fume has significant effects on the residual compressive strength. The greatest relative residual strength losses of concrete HPC2.5

and without silica fume were observed at 600°C, which were 24 and 2%.

Beyond 600°C, the concrete may lose the majority of these properties, i.e., there are properties that can cancel out, and one can say that the concrete has become

When temperature increases beyond 400°C, the concrete strength decreases more rapidly due to the degradation of calcium silicate hydrate (C-S-H). The second

The results of the porosity for the HPC after various heat treatments ranging

• For all high-performance concretes, a monotonic and fairly regular increase in

• For CR2.5, the porosity values are higher than that of the HPC for all the

Between 20 and 200°C, the porosity increases very little. The HPC shows a decrease of 0.26%. Kalifa explains that the decrease in the porosity of HPC is associated with the densification due to the complementary hydration of HSC.

phase of the C-S-H decomposes in the temperature range from 600 to 800°C forming β-C2S [16]. At a temperature of 900°C, the C-S-H breaks down completely. Therefore, the critical temperature for concrete ranges from approximately

400–900°C. In this range concrete loses most of its strength.

from 20 to 900°C are shown in **Figure 6**.

porosity with temperature is observed.

*DOI: http://dx.doi.org/10.5772/intechopen.89916*

**Figure 5.** *Compressive strength of (HPC2.5) and (CR2.5) with temperatures [18].*

*Mechanical Behavior of High-Performance Concrete under Thermal Effect DOI: http://dx.doi.org/10.5772/intechopen.89916*

At 600°C, the quick losses in compressive strength for HPC2.5 concretes are attributed to the dense microstructure in this type of concretes, which caused the buildup of higher internal pressure due to the water vapor transition of the interlayer water. As a result, this process as well as chemical decomposition of hydration products causes severe deteriorations and strength loses in concrete after subjecting to high temperatures. It seems that the dosage of silica fume has no significant effect on the relative residual compressive strength at 200°C. However, between 200 and 400°C, the amount of 5% of silica fume has significant effects on the residual compressive strength. The greatest relative residual strength losses of concrete HPC2.5 and without silica fume were observed at 600°C, which were 24 and 2%.

Beyond 600°C, the concrete may lose the majority of these properties, i.e., there are properties that can cancel out, and one can say that the concrete has become weak.

When temperature increases beyond 400°C, the concrete strength decreases more rapidly due to the degradation of calcium silicate hydrate (C-S-H). The second phase of the C-S-H decomposes in the temperature range from 600 to 800°C forming β-C2S [16]. At a temperature of 900°C, the C-S-H breaks down completely. Therefore, the critical temperature for concrete ranges from approximately 400–900°C. In this range concrete loses most of its strength.
